DOI: 10.17188/1286085
title: Materials Data on Rb10NaAl11Si13O48 by Materials Project

description: Rb10NaAl11Si13O48 crystallizes in the triclinic P1 space group. The structure is three-dimensional. there are ten inequivalent Rb sites. In the first Rb site, Rb is bonded in a 1-coordinate geometry to two O atoms. There are one shorter (2.81 Å) and one longer (3.00 Å) Rb–O bond lengths. In the second Rb site, Rb is bonded in a 6-coordinate geometry to six O atoms. There are a spread of Rb–O bond distances ranging from 2.70–3.26 Å. In the third Rb site, Rb is bonded in a 6-coordinate geometry to six O atoms. There are a spread of Rb–O bond distances ranging from 2.76–3.24 Å. In the fourth Rb site, Rb is bonded to five O atoms to form distorted RbO5 trigonal bipyramids that share corners with two SiO4 tetrahedra and edges with four AlO4 tetrahedra. There are a spread of Rb–O bond distances ranging from 2.84–3.25 Å. In the fifth Rb site, Rb is bonded in a 5-coordinate geometry to five O atoms. There are a spread of Rb–O bond distances ranging from 2.94–3.26 Å. In the sixth Rb site, Rb is bonded in a 3-coordinate geometry to five O atoms. There are a spread of Rb–O bond distances ranging from 2.58–3.30 Å. In the seventh Rb site, Rb is bonded in a 5-coordinate geometry to five O atoms. There are a spread of Rb–O bond distances ranging from 2.70–3.22 Å. In the eighth Rb site, Rb is bonded in a 5-coordinate geometry to five O atoms. There are a spread of Rb–O bond distances ranging from 2.74–3.06 Å. In the ninth Rb site, Rb is bonded in a 1-coordinate geometry to one O atom. The Rb–O bond length is 2.61 Å. In the tenth Rb site, Rb is bonded in a 3-coordinate geometry to three O atoms. There are a spread of Rb–O bond distances ranging from 2.82–3.28 Å. Na is bonded in a distorted trigonal non-coplanar geometry to three O atoms. There are a spread of Na–O bond distances ranging from 2.23–2.31 Å. There are eleven inequivalent Al sites. In the first Al site, Al is bonded to four O atoms to form AlO4 tetrahedra that share corners with two AlO4 tetrahedra and corners with two SiO4 tetrahedra. There are a spread of Al–O bond distances ranging from 1.75–1.79 Å. In the second Al site, Al is bonded to four O atoms to form AlO4 tetrahedra that share a cornercorner with one AlO4 tetrahedra and corners with three SiO4 tetrahedra. There are a spread of Al–O bond distances ranging from 1.73–1.80 Å. In the third Al site, Al is bonded to four O atoms to form AlO4 tetrahedra that share a cornercorner with one SiO4 tetrahedra, corners with three AlO4 tetrahedra, and an edgeedge with one RbO5 trigonal bipyramid. There are a spread of Al–O bond distances ranging from 1.72–1.82 Å. In the fourth Al site, Al is bonded to four O atoms to form AlO4 tetrahedra that share a cornercorner with one SiO4 tetrahedra and corners with three AlO4 tetrahedra. There are a spread of Al–O bond distances ranging from 1.73–1.82 Å. In the fifth Al site, Al is bonded to four O atoms to form AlO4 tetrahedra that share a cornercorner with one SiO4 tetrahedra, corners with three AlO4 tetrahedra, and an edgeedge with one RbO5 trigonal bipyramid. There are a spread of Al–O bond distances ranging from 1.74–1.80 Å. In the sixth Al site, Al is bonded to four O atoms to form corner-sharing AlO4 tetrahedra. There are a spread of Al–O bond distances ranging from 1.73–1.79 Å. In the seventh Al site, Al is bonded to four O atoms to form AlO4 tetrahedra that share corners with two AlO4 tetrahedra, corners with two SiO4 tetrahedra, and an edgeedge with one RbO5 trigonal bipyramid. There are a spread of Al–O bond distances ranging from 1.70–1.83 Å. In the eighth Al site, Al is bonded to four O atoms to form AlO4 tetrahedra that share a cornercorner with one SiO4 tetrahedra, corners with three AlO4 tetrahedra, and an edgeedge with one RbO5 trigonal bipyramid. There are a spread of Al–O bond distances ranging from 1.72–1.80 Å. In the ninth Al site, Al is bonded to four O atoms to form AlO4 tetrahedra that share corners with two AlO4 tetrahedra and corners with two SiO4 tetrahedra. There are a spread of Al–O bond distances ranging from 1.70–1.83 Å. In the tenth Al site, Al is bonded to four O atoms to form AlO4 tetrahedra that share a cornercorner with one SiO4 tetrahedra and corners with three AlO4 tetrahedra. There are a spread of Al–O bond distances ranging from 1.71–1.80 Å. In the eleventh Al site, Al is bonded to four O atoms to form AlO4 tetrahedra that share corners with two AlO4 tetrahedra and corners with two SiO4 tetrahedra. There are a spread of Al–O bond distances ranging from 1.74–1.78 Å. There are thirteen inequivalent Si sites. In the first Si site, Si is bonded to four O atoms to form corner-sharing SiO4 tetrahedra. There are a spread of Si–O bond distances ranging from 1.61–1.65 Å. In the second Si site, Si is bonded to four O atoms to form SiO4 tetrahedra that share a cornercorner with one AlO4 tetrahedra and corners with three SiO4 tetrahedra. There are a spread of Si–O bond distances ranging from 1.61–1.67 Å. In the third Si site, Si is bonded to four O atoms to form corner-sharing SiO4 tetrahedra. There are a spread of Si–O bond distances ranging from 1.60–1.65 Å. In the fourth Si site, Si is bonded to four O atoms to form SiO4 tetrahedra that share corners with two AlO4 tetrahedra and corners with two SiO4 tetrahedra. There are a spread of Si–O bond distances ranging from 1.60–1.67 Å. In the fifth Si site, Si is bonded to four O atoms to form SiO4 tetrahedra that share corners with two AlO4 tetrahedra, corners with two SiO4 tetrahedra, and a cornercorner with one RbO5 trigonal bipyramid. There are a spread of Si–O bond distances ranging from 1.62–1.66 Å. In the sixth Si site, Si is bonded to four O atoms to form SiO4 tetrahedra that share a cornercorner with one AlO4 tetrahedra and corners with three SiO4 tetrahedra. There are a spread of Si–O bond distances ranging from 1.61–1.65 Å. In the seventh Si site, Si is bonded to four O atoms to form SiO4 tetrahedra that share corners with two AlO4 tetrahedra, corners with two SiO4 tetrahedra, and a cornercorner with one RbO5 trigonal bipyramid. There are a spread of Si–O bond distances ranging from 1.62–1.66 Å. In the eighth Si site, Si is bonded to four O atoms to form SiO4 tetrahedra that share a cornercorner with one AlO4 tetrahedra and corners with three SiO4 tetrahedra. There are a spread of Si–O bond distances ranging from 1.62–1.65 Å. In the ninth Si site, Si is bonded to four O atoms to form SiO4 tetrahedra that share a cornercorner with one AlO4 tetrahedra and corners with three SiO4 tetrahedra. There are a spread of Si–O bond distances ranging from 1.59–1.67 Å. In the tenth Si site, Si is bonded to four O atoms to form SiO4 tetrahedra that share a cornercorner with one AlO4 tetrahedra and corners with three SiO4 tetrahedra. There are a spread of Si–O bond distances ranging from 1.62–1.65 Å. In the eleventh Si site, Si is bonded to four O atoms to form SiO4 tetrahedra that share corners with two AlO4 tetrahedra and corners with two SiO4 tetrahedra. There are a spread of Si–O bond distances ranging from 1.61–1.65 Å. In the twelfth Si site, Si is bonded to four O atoms to form SiO4 tetrahedra that share a cornercorner with one AlO4 tetrahedra and corners with three SiO4 tetrahedra. There are a spread of Si–O bond distances ranging from 1.59–1.67 Å. In the thirteenth Si site, Si is bonded to four O atoms to form SiO4 tetrahedra that share corners with two AlO4 tetrahedra and corners with two SiO4 tetrahedra. There are a spread of Si–O bond distances ranging from 1.60–1.68 Å. There are forty-eight inequivalent O sites. In the first O site, O is bonded in a bent 150 degrees geometry to two Si atoms. In the second O site, O is bonded in a distorted bent 150 degrees geometry to two Si atoms. In the third O site, O is bonded in a bent 150 degrees geometry to two Si atoms. In the fourth O site, O is bonded in a bent 150 degrees geometry to one Rb and two Si atoms. In the fifth O site, O is bonded in a distorted bent 150 degrees geometry to one Rb, one Al, and one Si atom. In the sixth O site, O is bonded in a bent 150 degrees geometry to one Al and one Si atom. In the seventh O site, O is bonded in a 2-coordinate geometry to two Rb and two Al atoms. In the eighth O site, O is bonded in a bent 150 degrees geometry to two Si atoms. In the ninth O site, O is bonded in a bent 150 degrees geometry to two Si atoms. In the tenth O site, O is bonded in a bent 150 degrees geometry to two Si atoms. In the eleventh O site, O is bonded in a distorted bent 150 degrees geometry to one Rb and two Si atoms. In the twelfth O site, O is bonded in a bent 150 degrees geometry to two Si atoms. In the thirteenth O site, O is bonded in a distorted bent 150 degrees geometry to one Rb and two Si atoms. In the fourteenth O site, O is bonded in a distorted bent 150 degrees geometry to one Rb, one Al, and one Si atom. In the fifteenth O site, O is bonded in a distorted bent 150 degrees geometry to one Rb, one Al, and one Si atom. In the sixteenth O site, O is bonded in a bent 120 degrees geometry to two Si atoms. In the seventeenth O site, O is bonded in a bent 120 degrees geometry to two Si atoms. In the eighteenth O site, O is bonded in a linear geometry to one Rb and two Si atoms. In the nineteenth O site, O is bonded in a linear geometry to two Si atoms. In the twentieth O site, O is bonded in a linear geometry to one Rb and two Si atoms. In the twenty-first O site, O is bonded in a linear geometry to two Rb, one Al, and one Si atom. In the twenty-second O site, O is bonded in a linear geometry to two Si atoms. In the twenty-third O site, O is bonded in a bent 150 degrees geometry to two Si atoms. In the twenty-fourth O site, O is bonded in a distorted bent 150 degrees geometry to one Rb, one Al, and one Si atom. In the twenty-fifth O site, O is bonded in a distorted bent 150 degrees geometry to one Rb, one Al, and one Si atom. In the twenty-sixth O site, O is bonded in a bent 120 degrees geometry to one Rb, one Al, and one Si atom. In the twenty-seventh O site, O is bonded in a bent 120 degrees geometry to one Rb, one Al, and one Si atom. In the twenty-eighth O site, O is bonded in a distorted bent 120 degrees geometry to one Rb, one Al, and one Si atom. In the twenty-ninth O site, O is bonded in a distorted bent 120 degrees geometry to one Rb and two Al atoms. In the thirtieth O site, O is bonded in a 3-coordinate geometry to one Rb and two Al atoms. In the thirty-first O site, O is bonded in a distorted bent 150 degrees geometry to one Rb and two Al atoms. In the thirty-second O site, O is bonded in a distorted T-shaped geometry to one Rb and two Al atoms. In the thirty-third O site, O is bonded in a 4-coordinate geometry to one Rb, one Na, and two Al atoms. In the thirty-fourth O site, O is bonded in a distorted bent 150 degrees geometry to three Rb and two Al atoms. In the thirty-fifth O site, O is bonded in a distorted bent 150 degrees geometry to two Rb and two Al atoms. In the thirty-sixth O site, O is bonded in a distorted bent 150 degrees geometry to three Rb and two Al atoms. In the thirty-seventh O site, O is bonded in a distorted bent 150 degrees geometry to two Rb and two Al atoms. In the thirty-eighth O site, O is bonded in a distorted linear geometry to one Rb and two Al atoms. In the thirty-ninth O site, O is bonded in a distorted bent 150 degrees geometry to one Rb and two Al atoms. In the fortieth O site, O is bonded in a 2-coordinate geometry to two Rb, one Al, and one Si atom. In the forty-first O site, O is bonded in a distorted bent 150 degrees geometry to one Rb, one Al, and one Si atom. In the forty-second O site, O is bonded in a 4-coordinate geometry to two Rb, one Al, and one Si atom. In the forty-third O site, O is bonded in a 2-coordinate geometry to two Rb, one Al, and one Si atom. In the forty-fourth O site, O is bonded in a distorted bent 150 degrees geometry to one Rb, one Al, and one Si atom. In the forty-fifth O site, O is bonded in a 3-coord